Disclosure to Promote the Right To Information Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public. “जान1 का अ+धकार, जी1 का अ+धकार”
“प0रा1 को छोड न' 5 तरफ”
“The Right to Information, The Right to Live”
“Step Out From the Old to the New”
Mazdoor Kisan Shakti Sangathan
IS 2386-5 (1963): Methods of Test for Aggregates for Concrete, Part V: Soundness [CED 2: Cement and Concrete]
“!ान $ एक न' भारत का +नम-ण” Satyanarayan Gangaram Pitroda
“Invent a New India Using Knowledge”
“!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता ह” है” ह Bhartṛhari—Nītiśatakam
“Knowledge is such a treasure which cannot be stolen”
( Reaffirmed 2002 )
. .. .
\t. . . . . .
METHODS OF TEST FOR CONCRETE PART V Cement
Chairman SHRI K. K. NAMBIAR
I 1 / 1 !
and Concrete Sectional Committee, BDC 2 Representing The Concrete Association of India, Bombay
Members SHRI K. V. THADANEY ( Alternate to Shri K. K. Nambiar ) M. N. Dastur & Co. Private Ltd., Calcutta SHRI K. F. ANTIA Bhakra Dam Designs Directorate, New Delhi SHRI P. S. BHATNA~AR Central Water I_%Power Commission ( Ministry of DR. I. C. DOS M. PAIS CIJDDOU Irrigation t Power ) SHRI Y. K. MURTHY ( Alternate ) Khira Steel Works Private Ltd., Bombay SHRI N. D. DAFTARY Central Public Works Department SHRI N. G. DEWAN SUPER~ETENDIN~ENGINEER, END CIRCLE( Alternate ) The Associated Cement Companies Ltd., Bombay DR. R. R. HATTIBNQADI SHRI V. N. PAI ( Alternate ) Geological Survey of India, Calcutta SHRI P. C. HAZRA JOINT DIRECTOR STANDARDS Research, Designs & Standards Organization ( Ministry of Railways ) (B&S) ASSISTANTDIRECTORSTANDARDS ( B & S ) ( Alternate ) S. B. Joshi & Co. Private Ltd., Bombay SHRI S. B. JOSHI U. P. Government Cement Factory, Churk &RI M. M. LAL Directorate General of Supplies 8~.Disposals ( MinisSHRI B. N. MAJU~DAR try of Economic t Defence Co-ordination ) SHRI P. L. DAS ( Alternate ) CentrD;;hyd Research Institute ( CSIR ), New PROF. S. R. MEHRA The Concrete Association of India, Bombay SRRI N. H. MOHILE Government Test House, Calcutta SHRI S. N. MUKERJI SHRI N. C. SEN GUPTA ( Alternate ) Institution of Engineers ( India ), Calcutta SHRI ERACH A. NADIRSHAH National Buildings Organisation ( Minist,ry of SHRI C. B. PAT& Works, Housing & Rehabilitation ) SHRI RABINDER SINC+H (Alternate) Cent~~or~~~lding Research Institute ( CSIR ), PR0F.G. S.RAMASWAMY SHRIK. SIVAPRASAD( Alternate) Gammon India Limited, Bombay SHRI T. N. S. RAO SHRI S.R. PINHEIRO (Alternate)
( Continued on page 2) INDIAN STANDARDS INSTITUTION MANAK BHAVAN, 9 MATHURA ROAD NEW DELHI 1
is.2 23&l (RR* V:) - 1%3 ( Cot&wed from page 1)
Martin Burn Ltd.. Calcutta Dslmia Cement ( Bharat ) Ltd., Calcutta Central ‘Board of Irrigetion & Power ( Ministry of Irrigation & Power ) Engineer-in-Chief’s Branch, Army~Headquarters
REPRESENTATIVE SHRI NIHAR CnANDnA ROY SECRETARY
BRIG G. S. SIHOTA ’ SHRI R. S. MEIIANDRU ( Alternate ) Indian Roads Congress, New Delhi DR. BH. SUBBARAJU Roads Wing, Ministry of Transport SHRI J. M. TREHAN cations SHRI N. H. KESWANI ( Alternute ) Director, IS1 ( Ex-officio Member ) DR. H. C. VISVESVABAYA, Deputy Director ( Bldg )
SHRI A. PRITHIVI RAJ Assistant Director ( Bldg ), IS1
Concrete Subcommittee, BDC 2 : 2 Convener
Saab S . B . JOSHI
ASSISTANT DIRECTOR STANDARDS ( B & S ) SHRI N. H. BHAQWANANI DR. I. C. DOS M. PAIS CUDDOU
S. B. Joshi & Co. Private
Designs & Standards Organization Resee& ( Ministry of Railways ) Engineer-in-Chief’s Branch, Army Headquarters Central Water & Power Ccmmission (Ministry of Irrigation & Power )
SHRI Y. K; MURTHY ( Alternate ) Directorate SHRI P. I,. D_4s ii::7
General of Supplies & Disposals of Economic & Defence Co-ordina-
SHR~ B. N. MAJUMDAR ( Alternate ) Engineering Research Laboratory, Hyderabad DIRECTOR Mahsrashtra Public Works Department SHRI V. N. GUNAJI National Buildings Orgrtnisation ( Ministry of SHRI M. A. HAFEEZ Works, Housing & Rehabilitation ) SHRI B. S. SHIVAMURTHY ( Alternate ) Central Water & Power Commission ( Ministry of SHRI C. L. HANDA Irrigation & Power ) Geological Survey of India, Celoutta Sam P. C. HAZRA The Concrete Association of India, Bombay SHRI K. K. NAMBJAR SHRI C. L. N. IYEN~AR (Alternate ) Central Road Research Institute ( CSIR ), New DR. M. L. PURI Delhi Cent;lArz3ilding Research Institute ( CSIR ), PROF. G. S. RAMASWAMY SHRI K. SIVA PRASAD ( Alternate ) Gammon India Ltd., Bombay SHRI T. N. S. RAO SHRI S. R. PINHEIRO ( Alternate ) ENGINEER, Central Public Works Department SUPERINTENDING 2ND CIRCLE SHRI 0. P. GOEL ( Alternute ) Roads Wing, Ministry of Transport & CommunicaSHRI J. M. TRE~AN tions SRRI R. P. SI~KA ( AIternate ) Braithwaite Burn & Jessop Construction Co. Ltd., SHRI H. T. YAN Calcutta
Indian Standard METHODS OF TEST . FOR AGGREGATES FOR COWCRETE PART V
0.1This IndianStandard (Part V) was adopted by the Indian Standards Institution on 13 September 1963, after the draft finalized by the Cement and Concrete Sectional Committee had been approved by the Building Division Council. 0.2 One of the major contributing factors to the quality of concrete is the The test methods given in this standard quality of aggregates used therein. In a given are intended to assist in assessing the quality of aggregates. situation, for a particular aggregate, it may not be necessary to assess all the qualities, and therefore it is necessary to determine beforehand the purpose for which a concrete is being used and the qualities of the aggregate which require to be assessed. Accordingly, the relevant test methods may For the be chosen from amongst the various tests covered in this standard. convenience of the users, the test methods are grouped into the following eight parts of Indian Standard Methods of Test for Aggregates for Concrete ( IS : 2386 - 1963): Part I Part II Part III Part Part Part Part Part
IV V VI VII VIII
Particle Size and Shape of Deleterious Materials and Organic Estimation Impurities Specific Gravity, Density, Voids, Absorption and Bulking Mechanical Properties Soundness Measuring Mortar Making Properties of Fine Aggregate Alkali Aggregate Reactivity Petrographic Examination
0.3 The Sectional Committee responsible for the preparation of this standard has taken into consideration the views of concrete specialists, testing authorities, consumers and technologists and has related the standard to the practices followed in this country. Further, the need for international co-ordination among standards prevailing in different countries 3
IS :23S6 (-Part V ) - 1963 of the world has also been recognized. These considerations led the Sectional Committee to derive assistance from C88 - 61T Tentative Method of Test for Soundness of Aggregates by Use of Sodium Sulphate or Magnesium Sulphate issued by American Society for ,Testing and Materials. 0.4 Wherever a reference to any Indian Standard appears in this method, it shall be taken as a reference to its latest version. 0.5 For the purpose of deciding whether a particular requirkment of this standard is complied with, the final value, observed or calculated, expressing the result of a test or analysis, shall be rounded off in accordance with The IS : 2 - 1960 Rules for Rounding Off Numerical Values (Revised). number of significant places retained in the rounded off value should be the same as that of the specified value in this standard. 0.6 This standard is intended chiefly to cover the technical provisions relating to testing of aggregates for concrete, and it does not include all the necessary provisions of a contract.
I. SCOPE 1.1 This standard (Part V > covers the method of test to determine the resistance to disintegration of aggregates by saturated solutions of sodium sulphate or magnesium sulphate. NOTEThis test furnishes information helpful in judging the soundness of aggregates subject to weathering action, particularly when adequate information is not available from service records of the material exposed to actual weathering Attention is called to the fact that test results by the use of the two conditions. salts differ considerably, and care shall be exercised in fixing proper limits in any specification which may include requirements for these tests.
2. APPARATUS 2.1 Sieves - Sieves of the following sizes, having square openings, complying with the requirements specified in IS : 460 - 1962 Specification for Test Sieves (Revised ) shall be used: Coarse Series Fine Series 8.0 mm 150 microns 10 mm 300 microns 12.5 mm 16 mm 600 microns 20 mm 25 mm l-18 mm 31.5 mm 2.36 mm 40 mm 50 mm 4.00 mm 63 mm 475 mm 80 mm 4
IS:2386(PaktV)-1963 2.2 Containers - Containers for immersing the samplei of aggregate in the solution, in accordance with the procedure described in this method, shall be perforated in such a manner as to permit free access of the solution to the sample and drainage of the solution from the sample without loss of aggregate. Arrangements shall also be available to ensure that the volume of the solution in which samples are immersed shall be at least five times the volume of the sample immersed at any one time. NOTE -
Baskets made of suitable wire mesh or sieves with suitable
~ satisfactory containers for the samples.
means for regulating the 2.3 Temperature Regulation - Suitable temperature of the samples during immersion in the sodium sulphate or magnesium sulphate solution shall be provided. 2.4 Balances - For weighing fine aggregate, a balance having a capacity of not less than 500 g, sensitive to at least 0.1 g, shall be used; for weighing coarse aggregate, a balance having a capacity of not less than 5 000 g, sensitive to at least one gram, shall be used. 2.5 Drying Oven - The drying oven shall be capable of being maintained between 105” and 110°C and the rate of evaporation, at this range of temperature, shall average at least 25 g/h for four hcurs during which period the doors of the oven shall be kept closed. NOTE -- This rate shall be determined by the loss of water from 1-litre low-form beakers each initially containing 500 g of water at a temperature of 27” f 2°C placed at each corner and centre of each shelf of the oven. The evaporation requirement is to apply when the oven is empty except for the beakers of water.
3. REAGENTS 3.1 Sodium Sulphate Solution - Saturated solution of sodium sulphate shall be prepared by dissolving sodium sulphate, technical grade, conforming to IS : 255 - 1950 Specification for Sodium Sulphate, Anhydrous, Technical, or an equivalent grade of the salt of either the anhydrous (Na,SO,) or the crystalline ( Na,S04.10H,0)* form in water at a temperature of 25” to 30°C. Sufficient salt ( see Note ) shall be added to ensure not only saturation but aIso the presence of excess crystals when the solution is ready for use in the tests. The mixture shall be thoroughly stirred during the addition of the salt and the solution shall be stirred at frequent intervals until used. The solution shall be cooled to a temperature of 27” & 2°C and maintained at that temperature for at least 48 hours before use. The solution shall be thoroughly stirred immediately before *Experience with the test method indicates that a grade of sodium sulphate designated by the trade as dried powder, which may be considered as approximately anhydrous, is the most practical for use. That grade is more economically The decahydrate sodium sulphate presents available than the anhydrous form. difRculties in compounding the required solution on account of its cooling effect on the solution,
ISIt 2386 ( Part V ) - 1963 use and salt cakes, if any, shall be broken and the specific gravity shall be determined. When used, the solution shall have a specific gravity of not less than l-151 and not greater than 1,174. Discoloured solution shall be discarded, or filtered and checked for specific gravity. NOTE -For making up the solution, 350 g of anhydrous salt decahydrate salt per litre of water are sufficient for saturation at since these salts are not completely stable and since it is desirable crystals be present, the use of not less than 420 g of the anhydrous the decahydrate salt per litre of water is recommended.
or 1 150 g of the 28’C. However that an excess of salt or 1 300 g of
3.2 Magnesium Sulphate Solution - The saturated solution of magnesium sulphate shall be made by dissolving magnesium sulphate, technical grade, conforming to IS : 257 - 1950 Specification for Magnesium Sulphate (Epsom Salt ), Technical, or an equivalent grade of the salt of either the anhydrous ( MgSO, ) or the crystalline ( MgS0,.7H,O ) ( epsom salt ) form in water at a temperature of 25” to 30°C. Sufficient quantity of salt ( see Note ) shall be added to ensure ‘saturation and the presence of excess crystals when the solution is ready for use in the tests. The mixture shall be thoroughly stirred during the addition of the salt aud the solution shall be stirred at frequent intervals until used. The solution shall be cooled to a temperature of 27” & 1°C and maintained at that temperature for at least 48 hours before use. The solution shall be thoroughly stirred immediately before use and salt cakes, if any, shall be broken up and the specific gravity shall be determined. When used, the solution shall have a specific gravity of not less than 1.295 and not more than 1.308. Discoloured solution shall be discarded, or filtered and checked for specific gravity. NOTE - For making up the solution, 400 g of anhydrous salt or 1 400 g of the heptahydrate per litre of water are sufficient for saturation at 28°C. However, since these salts are not completely stable, with the hydrous salt being the more stable of the two, and since it is desirable that an excess of crystals be present, it is recommended that the heptahydrate salt be used and in an amount of not less than 1 600 g per litre of water.
4. SAMPLES 4.1 Fine Aggregate - Fine aggregate for the test shall be passed through a lo-mm IS Sieve. The sample sh@l be of such a size that it will yield not less than 100 g of each of the following sizes, which shall be available in amounts of 5 percent or more, expressed in terms of the following sieves:
Passing IS Sieve
Retained on IS Sieve
1*18-mm 2*36-mm &75-mm
600-micron 1.18-mm 2.36mm
IS:2386(PartV)-1963 4.2 Coarse Aggregate - Coarse aggregate for the test shall consist of material from which sizes finer than 475mm IS Sieve have been removed; such sizes shall be tested in accordance with the procedure for fine aggregate. The sample shall be of such a size that it will yield not less than the following amounts of the different sizes, which shall be available in amounts of 5 percent or more:
Size ( Square-Hole Sieves ) 10 mm to 4.75 mm 20 mm to 10 mm consisting of: 12.5 mm to 10 mm 20 mm to 12.5 mm 40 mm to 20 mm consisting of: 25 mm to 20 mm 40 mm to 25 mm 63 mm to 40 mm consisting of: 50 mm to 40 mm 63 mm to 50 mm 80 mm and larger sizes by 20 mm spread in sieve size, each fraction
Yield 300 g 1 000 g 33 percent 67 percent 1 500 g 33 percent 67 percent 3 000 g 50 percent 50 percent 3 000 g
4.3 All-h-Aggregate - All-in-aggregate shall be separated in two major fractions, finer than 4.75 mm and coarser than 4.75 mm. The former shall be dealt with as fine aggregate and the latter as coarse aggregate. NOTE -It shall be noted that testing closely sized aggregates, such as these constitutes a more severe test than testing a graded aggregate, and this fact should be taken into account while specifying limits in specifications.
4.4 Should the samples contain less than 5 percent of any of the sizes specified in 4.1 or 4.2, that size shall not be tested, but, for the purpose of calculating the test result, it shall be considered to have the same loss in sodium sulphate or magnesium sulphate treatment as the average of the next smaller and the next larger size, or if one of these sizes is absent, it shall be considered to have the same loss as the next larger or next smaller size, whichever is present. When the 20 mm to 10 mm, 40 mm to 20 mm or 63 mm to 40 mm test samples specified in 4.2 cannot be prepared due to the absence of one or two sizes of aggregate shown for each, the size available shall be used to prepare the sample tested. 5. PREPARATION
5.1 Fine Aggregate - The sample of fine aggregate shall be thoroughly washed on a 300-micron IS Sieve, dried to constant weight at 105â€? to 110Â°C
and separated into different sizes by sieving as follows: Make a rough separation of the graded sample by means of a nest of the,sieves specified in 4.1. From the fractions obtained in this manner, select samples of sufficient size to yield 100 g after sieving to refusal. (In general, a 110 g sample will be sufficient.) Fine aggregate sticking in the meshes of the sieves shall not be used in preparing the samples. Samples of 100 g shall be weighed out of each of the separated fractions after final sieving and placed in separate containers for the test. 5.2 Coarse Aggregate - The sample of coarse aggregate shall be thoroughly washed and dried to constant weight at 105°C to 110°C and shall be separated into different sizes shown in 4.2 by sieving to refusal. The proper weight of sample for each fraction shall be weighed out and placed in separate containers for the test. In the case of fractions coarser than the 20-mm IS Sieve, the number of particles shall also be counted. 6. PROCEDURE 6.1 Storage of Samples in Solution - The samples shall be immersed in the prepared solution of sodium sulphate or magnesium sulphate for not less than 16 hours nor more than 18 hours in such a manner that the solution covers them to a depth of at least 15 mm (see Note ). The containers shall be covered to reduce evaporation and prevent the accidental The samples immersed in the solution addition of extraneous substances. shall be maintained at a temperature of 27” & 1°C for the immersion period. NOTE Suitably weighted wire grids placed over the sample in the containers will permit this coverage to be achieved with very light aggregates.
6.2 Drying Samples After Immersion -After the immersion period, the aggregate sample shall be removed from the solution, permitted to drain for 15 f 5 minutes, and placed in the drying oven. The temperature of the oven shall have been brought previously to 105” to 110°C. The samples shall be dried to constant weight at this specified temperature. During the drying period, the samples shall be removed from the oven, cooled to room temperature and weighed at intervals of not less than 4 hours nor more than 18 hours. Constant weight may be considered to have been achieved when two successive weights for any one sample differ by less than 0.1 g in the case of fine aggregate samples, or by less than 1.0 g in the case of coarse aggregate samples. After constant weight has been achieved the samples shall be allowed to cool to room temperature, then they shall again be immersed in the prepared solution as described in 6.1.
6.3 Number of Cycles - The process of alternate immersion and drying shall be repeated until the specified number of cycles as agreed to between the purchaser and the vendor is obtained. 8
7. QUANTITATIVE BCAMINATION 7.1 The quantitative examination (see Note) shall be made as follows: a) After the completion of the final cycle and after the sample has cooled, the sample shall be washed free from the sodium sulphate or magnesium sulphate as determined by the reaction of the washwater with barium chloride ( BaCl, ). b) After the sodium sulphate or magnesium sulphate solution has been removed, each fraction of the sample shall be dried to constant weight at 105â€? to 110X, and weighed, Fine aggregates shall be sieved over the same sieve on which it was retained before the test, and coarse aggregate over the sieve shown below for the appropriate size of particle:
Size of Aggregate 63 mm to 40 mm to 20mmto 10 mm to
Sieve Used to Determine Loss
40 mm 20 mm 10mm 475 mm
31.5 mm 16 mm 80 mm 4.00 mm
NOTE-In addition to the procedure described in (a) and (b), it is suggested that additional information of value will be obtained by examining each fraction visually in order to determine whether there is any evidence of excessive splitting of the It is also suggested that additional information of value will be obtained grains. if, after treating each separate fraction of the sample as described in (b), all sizes, including detritus, are combined and a sieve analysis made using sieves of the following sizes:
150,300 and 800 micron, 1*18,2*36, 4.75, 10,20,40, and 80 mm. The results of the sieve analysis shall be recorded as cumulative retained on each sieve. 8.
of samples coarser than 20 mm shall be examined qualjtatively after each immersion and quantitatively at the completion of the test. 8.2 The qualitative examination and record shall consist of two parts, (a) observing the effect of the action (see Note ) by the sodium sulphate or magnesium sulphate solution and the nature of the action, and (b) counting the number of particles affected. NOTE--Many types of actions may b,e expected. In general, they may be classified as disintegration, splitting, crumbling, cracking, flaking, etc. While only particles larger than 20 mm in size are required to be examined qualitatively, it is recommended that examination of the smaller sizes be also made in order to determine whether there is any evidence of excessive splitting. 9.
REPORTING OF RESULTS
9.1 The report shall include the following data: a) Weight of each fraction
sample before test.
IS:2386(PartV)-1963 b) Material from each fraction of the sample finer than the sieve on which the fraction was retained before test, expressed as a percentage by weight of the fraction. c) Weighted average calculated from the percentage of loss for each fraction, based on the grading of the sample as received for examination or, preferably, on the average grading of the material from that portion of the supply of which the sample is representative. In these calculations sizes finer than the 300-micron IS Sieve shall be assumed to have zero percent loss. In the case of particles coarser than 20 mm before test, (1) the number of particles in each fraction before test, and (2) the number of particles affected, classified as to number disintegrating, splitting, crumbling, cracking, flaking, etc. 4 Character of solution ( sodium sulphate or magnesium sulphate ). 9.2 A recommended form for recording of test data is given in Table I. Test values given are for illustration and these may be appropriate for either salt depending on the quality of the aggregate. TABLE I SUGGESTED FORM FOR RECORDING SOUNDNESS TEST DATA ( With Illustrative Test V+dues ) SIEVE SIZE ~___--L--_-~ Retained Passing on
150micron 300 1, 600 l*li)‘mm 2’36 ,: 4’75 ,, 10 mm Total
GRADINQOF ORIGINAL SAMPLE PERCENT
150 micron 300 ,, 600 I*lgmm 2.36 ,, 4’75 ,, -
WEIUHT OF TEST FRACTIONSBEFORE TEST
PERCENTAQE WEIGHTED PAsSINo AVERMXG FINER SIEVE (CORRECTED AFTER TEST PERCENT ( ACTUALPERLoss) CENTLOSS)
Soundness Test for Fine Aggregate 5’0 100 100 100 100 -
11.4 26.0 25’2 17.0 10’8 4’6
400 -_- ..___._~
z2 4.8 8.0 11.2 11*2*
1.09 1.21 1.36 1.21 0,52
4.8 8’0 9’6 11.2
0’96 3.60 2.20 1.34
Soundness Test for Coarse Aggregate 63 mm
40 ,, 20 ,, 10 I, Total
40 mm 20 ,? 10 ,, 4’75 ,, --
20’0 45.0 23.0 12’0
3 ooot 1500t _1 ooot 300t
*The percentage loss ( 11’2 percent ) of the next smaller size is used as the percentage loss for this size, since this size contains less than 5 percent of the original sample as received ( see 4.4 ) . tMinimum amounts; larger samples may be used.
Published on Mar 10, 2018